mix design of fiber reinforced concretes - ?· • glass fibres – substantial strengths 700 –...
Post on 04-Aug-2018
Embed Size (px)
Mix design of fiber reinforced concretesExercise 9
The poor tensile strength of concrete can be improved by the use of fibers
The fibres act as reinforcing in reinforcedconcrete - only in a different scale. The effectis denser but shorter
Their main purpose is to increase the energy absorption capacity and toughness of the material, but also increase tensile and flexural strength of concrete
There is considerable improvement in the post-cracking behavior of concretes containing fibers. Although in the fiber-reinforced concrete the ultimate tensile strengths do not increase appreciably, the tensile strains at rupture do.
Compared to plain concrete, fiber reinforced concrete is much tougher and more resistant to impact.
Plain concrete fails suddenly once the deflection corresponding to the ultimate flexural strength is exceeded; on the other hand, fiber-reinforced concrete continue to sustain considerable loads even at deflections considerably in excess of the fracture deflection of the plain concrete
F. A Mirza & P. Soroushianb 2002: Effects of alkali-resistant glass fiber reinforcement on crack and temperature resistance of lightweight concrete. Cement and Concrete CompositesVol 24, No 2, pp.223227
Areas of Application thin sheets roof tiles pipes panels shotcrete (ruiskubetoni) curtain walls (ei-kantavat (ulko)seint) ground slabs precast elements composite decks Impact resisting structures floors
Fibre materials: Steel
substantial strengths 500-2000 N/mm2 and modulus of elasticity 200 N/mm2
Adhesion improved by the shaping of the fibres Glass fibres
substantial strengths 700 4000 N/mm2 and modulus of elasticity 70 Gpa
Adhesion is not as good as with steel fibres Long term durability/resistance is a problem -> coating
Polypropylene, polyethene and other plastics Low strengths 100 N/m2 and even lower modulus of
elasticity 5 N/mm2
CE marking per directive 93/68/EC)
Name and address of the manufacturer
The last two numbers of the yearwhen the marking was made
Reference to the european standard
Description of the product: common name, purpose of use, group, measurements, shape tensile strength and effect on consistence
The manufacturer of the fibre must specify the minimum amount of fibres for achievingresidual flexural tensile strength of 1,5 MPa in crack mouth opening displacement of 0,5 mm and residual tensile strength of 1 MPa in crack mouth opening displacement of 3,5 mm
Amount of fibres Distribution of the fibres Orientation of the fibres Material properties:
Tensile strength modulus of elasticity
Shape of the fibre Slenderness ratio (hoikkuusluku) Properties of the concrete
Maximum size of aggregate Strength of the concrete Amount of cement
Slenderness ratio (hoikkuusluku)
The slenderness ratio can serve as a measure of stiffness:
Slenderness ratio =
Examination of fractured specimens of fiber-reinforced concrete shows that failure takes place primarily due to fiber pull-out or debonding. Thus unlike plain concrete, a fiber-reinforced
concrete specimen does not break immediately after initiation of the first crack.
This has the effect of increasing the toughness The failure mechanism is by pull-out.
you never exceed the tensile strength of the fiber. Bond is much weaker.
The addition of any type of fibers to plain concrete reduces the workability.
Concrete mixtures containing fibers posses very low consistencies. However, the placeability and compactability of concrete is much better than reflected by the low consistency.
Fibre reinforced concretes can, in general, be produced using conventional concrete practice, though there are some important differences. The basic problem is to introduce a sufficient volume of uniformly dispersed fibres in order to achieve the desired improvements in mechanical behaviour, while retaining sufficient workability in the fresh mix.
The performance of the hardened concrete is enhanced more by fibres with a higher aspect ratio, since this improves the fibre-matrix bond. On the other hand, a high aspect ratio adversely affects the workability of the fresh mix. In general, the problems of both workability and uniform distribution increase with increasing fibre length and volume Aspect Ratio = Length / Diameter Typical aspect ratios range from about 30 to 150. Maximum usage of fibres: 2% by volume.
J. Endgington, D.J. Hannant & R.I.T. Williams, Steel fiberreinforced concrete Current paper CP 69/74 Building research establishment Garston Watford 1974
One of the chief difficulties in obtaining a uniform fibre distribution is the tendency for the fibres to ball or clump together. Clumping may be caused by a number of factors:I. The fibres may already be clumped together
before they are added to the mix; normal mixing action will not break down these clumps.
II. Fibres may be added too quickly to allow them to disperse in the mixer.
III. Too high a volume of fibres may be added.IV. The mixer itself may be too worn or inefficient
to disperse the fibres.V. Introducing the fibres to the mixer before the
other concrete ingredients will cause them to clump together
Most commonly the fibres should be added last to the wet concrete.
The concrete typically should have a slump of 50-75 mm greater than the desired slump of the fibre reinforced concrete
The use of collated fibres held together by a water-soluble sizing which dissolves during mixing largely eliminates the problem of clumping
High cement content Water reducing admixtures (superplasticizers) Small maximum size of aggregate Fibers (1-2% by volume)
Fiber-reinforced concrete is generally made with a high cement content and low water/cement ratio.